- 45 Views
- Uploaded on
- Presentation posted in: General

Noise Modeling at Quantum Level for Multi-Stack Gate Dielectric MOSFETs .

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Zeynep Çelik-Butler

Industrial Liaisons:Ajit Shanware, Luigi Colombo, Keith Green, TI; Hsing-Huang Tseng, SEMATECH, Ania Zlotnicka, Freescale

Students:

Bigang Min, Siva Prasad Devireddy, Tanvir Morshed, Shahriar Rahman

University of Texas at Arlington

P. O. BOX 19072

Arlington, TX 76019

UTA Noise and Reliability Laboratory

- Noise Modeling
- Unified Flicker Noise Model
- Multi-Stack Unified Noise Model (MSUN)

- Experimental Verification
- Metal-Gated HfO2/SiO2 NMOSFETs – different interfacial layer processing
- Poly-Gated HfSiON/SiON NMOSFETs – variable interfacial layer thickness

- Conclusions and Future Work

UTA Noise and Reliability Laboratory

Unified Flicker Noise Model*

- Based on correlated number and mobility fluctuations theory.
- Equi-energy tunneling process.
- Traps in the gate dielectric trap/de-trap channel carriers
- Trapping/de-trapping phenomenon causes fluctuations in the carrier number.
- Fluctuations in carrier mobility due to remote Coulomb scattering from trapped charge.
- Uniform distribution of traps in the gate dielectric with respect to distance and energy level.

*K. K. Hung, P. K. Ko, C. Hu, Y. C. Cheng, “A unified model for the flicker noise in metal-oxide-semiconductor field-effect transistors,”IEEE Trans. Electron Devices, vol. 37, pp.654-665, 1990.

UTA Noise and Reliability Laboratory

z

L

x

W

SiO2

Tox

y

Traps

Source

Drain

Substrate

Carriers

Physical Mechanism for Noise

Channel carriers tunnel back and forth from the traps in the gate oxide causing fluctuations in the number of carriers. By virtue of Coulomb scattering from oxide trapped charges there are fluctuations in carrier mobility that cause additionalnoise in correlation with the carrier number fluctuations.

K. K. Hung, P. K. Ko, C. Hu, Y. C. Cheng, “A unified model for the flicker noise

in metal-oxide-semiconductor field-effect transistors,”

IEEE Trans. Electron Devices, vol. 37, pp.654-665, 1990.

UTA Noise and Reliability Laboratory

Unified Flicker Noise Model Expressions

K. K. Hung, P. K. Ko, C. Hu, and Y. C. Cheng

IEEE Trans. Electron Devices, vol. 37, pp.654-665,1990

BSIM Low Frequency Noise Model

UTA Noise and Reliability Laboratory

z

L

x

THK

W

High-k

y

TIL

Traps

x

y

z

Source

Drain

Substrate

Carriers

Interfacial layer

High-k Gate Stack Scenario

Channel carriers tunnel into the traps in high-k and interfacial layer causing fluctuations in carrier number and mobility in a correlated way.

The uniform dielectric trap density assumption does not hold.

The different trap profiles and various physical properties of high-k/interfacial layer materials like physical thicknesses, barrier heights etc. affect the 1/f noise.

UTA Noise and Reliability Laboratory

Multi-Stack Unified Noise Model (MSUN)

- Based on correlated number and mobility fluctuations theory
- Equi-energy tunneling process
- Traps in the gate dielectric layers trap/de-trap channel carriers
- Trapping/de-trapping phenomenon causes fluctuations in the carrier number
- Fluctuations in carrier mobility due to remote Coulomb scattering from trapped charge
- Scalable with regards to the high-k/interfacial layer physical thicknesses
- Takes different dielectric material properties into account
- Considers non-uniform distribution of traps in the high-k/interfacial layer with respect to distance and energy level

UTA Noise and Reliability Laboratory

NtIL0

Ec

exp(-γILz)

exp[-γHK(zTIL)]

Ei

Efn

Ev

THK

TIL

NtHK0

Typical Band Diagram for High-k Stack

Carrier tunneling probability into the gate dielectric is an exponentially decaying function with attenuation rates corresponding to the dielectric material.

NtIL0 – IL/Si interface trap density at intrinsic Fermi level

NtHK0– HK/IL interfacetrap density atintrinsic Fermi level

UTA Noise and Reliability Laboratory

Nt0 exp(ξ(Efn-Ei))

Nt(Efn) exp(ηz)

Nt(Efn)

Nt0

0

0

Ei

1.2

z

Trap Density Profile in SiO2

Nt0 exp(ξ(Efn-Ei))

=Nt(Efn)

Nt0 is the trap density at the Si/SiO2 interface and intrinsic Fermi level. Trap density increases exponentially towards the band edges at a rate defined by parameter ξ.

Nt(Efn)is the trap density at the Si/SiO2 interface and quasi-Fermi level. Trap density increases exponentially into the gate dielectric.

Z. Çelik-Butler, and T. Y. Hsiang, “Spectral dependence of 1/fγ noise on gate bias in n-MOSFETs,” Solid State Electron., vol. 30, pp. 419–423, 1987.

UTA Noise and Reliability Laboratory

NtIL0

Ec

Ei

Ef

Ev

NtHK0

High-K

Interfacial

Layer

Modified Trap Profile by Energy Band Bending

The energy bands bend in both high-k and interfacial layers due to the applied gate voltage. Higher trap density towards the band edges means that the trap profile encountered by channel carriers at a particular location in the dielectric is altered due to band bending. This effect is reflected by the parameters λIL and λHK.

Z. Çelik-Butler, and T. Y. Hsiang, “Spectral dependence of 1/fγ noise on gate bias in n-MOSFETs,” Solid State Electron., vol. 30, pp. 419–423, 1987.

UTA Noise and Reliability Laboratory

Trap density for (0<z<TIL)

Trap density for (TIL<z<THK+TIL)

UTA Noise and Reliability Laboratory

Power spectral density of the mean square fluctuations in the number of occupied trapsfor high-k/interfacial layer stack

Z. Çelik-Butler, “Different noise mechanisms in high-k dielectric gate stacks,” in Proc. SPIE—Noise and Fluctuations, pp. 177–184, 2005.

B. Min, S. P. Devireddy, Z. Çelik-Butler, A. Shanware, L. Colombo, K. Green, J. J. Chambers, M. R. Visokay, and A. L. P. Rotondaro,

“Impact of interfacial layer on low-frequency noise of HfSiON dielectric MOSFETs,” IEEE Trans. Electron Devices, vol. 53, pp. 1459–1466, 2006.

UTA Noise and Reliability Laboratory

- ft(1-ft) ensures that only traps within few kT of Efncontribute to fluctuations.
- Integral along the channel (x) approximated.
- The shape of the spectral density is modified from pure 1/f through functional form of Nt.
- Contribution to fluctuations from the high-k dielectric layer is much higher than that from the interfacial layer.

UTA Noise and Reliability Laboratory

After appropriate substitution of various parameters, the power spectral density of the mean square fluctuations can be written as

Conduction Band Offset with Si

Tunneling Coefficients

UTA Noise and Reliability Laboratory

Power spectral density for local current fluctuations

Total noise power spectral density

UTA Noise and Reliability Laboratory

- Noise Modeling
- Unified Flicker Noise Model
- Multi-Stack Unified Noise Model (MSUN)

- Experimental Verification
- Metal-Gated HfO2/SiO2 NMOSFETs – different interfacial layer processing
- Poly-Gated HfSiON/SiON NMOSFETs – variable interfacial layer thickness

- Conclusions and Future Work

UTA Noise and Reliability Laboratory

- Split C-V and DC Measurements
- 10µm 10µm devices
- 78K & 100K – 350K in steps of 25K (metal gate)
- 172K – 300K (poly gate)

- Noise and DC Measurements
- Metal gate
- 0.165µm 10µm devices
- 78K & 100K – 350K in steps of 25K

- Poly gate
- (0.20-0.25)µm 10µm devices
- 172K – 300K

- Metal gate
- Noise Modeling and Analysis
- Unified Flicker Noise Model
- Multi-Stack Unified Model

UTA Noise and Reliability Laboratory

UTA Noise and Reliability Laboratory

Normalized Noise vs. Temperature

Normalized noise for the two process splits shows no clear dependence on temperature at all bias points.

Generally, the magnitude of 10Å SRPO device is lower.

Metal-Gated HfO2/SiO2

UTA Noise and Reliability Laboratory

Parameter Extraction

The dependence of noise power

spectral density on frequency mainly

comes from the term,

where,

The frequency exponent for the

1-100Hz region is plotted against

the applied gate bias.

A straight line fit is made to the data

from which ηHK ,λHK are extracted

Metal-Gated HfO2/SiO2

UTA Noise and Reliability Laboratory

The trap density variation with respect to energy is represented as an exponentially varying function.

The energy interval swept by the quasi Fermi level for the temperature and the bias range considered in this work is 0.05eV.

Metal-Gated HfO2/SiO2

UTA Noise and Reliability Laboratory

MSUN Model

Metal-Gated HfO2/SiO2

UTA Noise and Reliability Laboratory

MSUN Model

Metal-Gated HfO2/SiO2

UTA Noise and Reliability Laboratory

Effective Oxide Trap Density vs. Temperature

Nt0HK is constant for all temperatures and the non-uniformity in trap density is modeled by ηHK ,λHK

MSUN Model

Metal-Gated HfO2/SiO2

UTA Noise and Reliability Laboratory

Effective Oxide Trap Density vs. Temperature

The overall effective trap density (Nt) is extracted using the Unified Flicker Noise Model.

In general, the values tend to increase with a decrease in temperature.

This is not consistent with the

uniform trap density assumption

at the core of the model.

Original Unified Noise Model

Metal-Gated HfO2/SiO2

UTA Noise and Reliability Laboratory

- Noise Modeling
- Unified Flicker Noise Model
- Multi-Stack Unified Noise Model (MSUN)

- Experimental Verification
- Metal-Gated HfO2/SiO2 NMOSFETs – different interfacial layer processing
- Poly-Gated HfSiON/SiON NMOSFETs – variable interfacial layer thickness

- Conclusions and Future Work

UTA Noise and Reliability Laboratory

- NMOS HfSiON with same high-k thickness (3.0 nm) and different interfacial layers (IL)

UTA Noise and Reliability Laboratory

- Normalized current noise spectral density did not show any noticeable dependence on temperature.
- The observed noise behavior is not affected by any temperature sensitive process.
- Remote optical phonon scattering may not have a significant impact on low frequency noise characteristics although it has a profound effect on mobility behavior (presented last year).

Poly-Gated HfSiON / SiON

UTA Noise and Reliability Laboratory

Correlated Number and Mobility Fluctuation Model1:

Hooge’s Bulk Mobility Fluctuation Model9:

Correlated number and surface mobility fluctuation mechanism was observed to dominate for devices with different interfacial layer thicknesses in the experimental temperature range

Poly-Gated HfSiON / SiON

9 F.N. Hooge. IEEE Trans. Electron Devices 41. 1926 (1994).

UTA Noise and Reliability Laboratory

According to original Unified Model, current noise spectral density can be shown as

(1)

Considering tunneling through a double step barrier, we can show

(2)

The final expression of Sid(A2/Hz) using the new model for high-k gate devices becomes

(3)

UTA Noise and Reliability Laboratory

- If the published trap density values are chosen for NtIL0 and NtHK0 the noise contribution of the interfacial layer is
- insignificant when compared to the total device noise. The interfacial layer parameters do not play any
- effective role in the data fitting
- For the high-k layer, as discussed earlier, λHK= ξHK, so the number of effective fitting parameters reduce to 4.

UTA Noise and Reliability Laboratory

From Eq (3) we can show

α=

From a linear fit of α as a function of

Vg for individual devices at all

temperatures, the energy dependence

parameters ξ, λ and the spatial

distribution parameter η were

extracted. The extracted values

are shown on the plots.

Poly-Gated HfSiON / SiON

UTA Noise and Reliability Laboratory

Poly-Gated HfSiON / SiON

The calculated current noise spectral density SId is compared to the data for devices with

four different IL thicknesses and in the experimental temperature range of 172K-300K.

UTA Noise and Reliability Laboratory

Poly-Gated HfSiON / SiON

Excellent agreement between data and model predictions was observed irrespective of IL thickness at all temperatures.

UTA Noise and Reliability Laboratory

SId (A2/Hz)

α=0

α~1

α~2

Frequency (Hz)

A special phenomena was observed for the

devices with the thickest gate oxide.

The higher frequency components in the device noise are contributed by traps closer to the interface, where as the traps further away contribute to the lower frequency components.

For the devices with TIL=1.8nm, the characteristic corner frequency was calculated to be fc2~ 33Hz. Below 33 Hz the noise was contributed by the high-k layer. Above this limit noise contribution was primarily from the IL layer.

UTA Noise and Reliability Laboratory

- The fit was good in the bias range of moderate inversion to strong inversion, for devices with all different IL thick-nesses in the experimental temperature range.

Poly-Gated HfSiON / SiON

UTA Noise and Reliability Laboratory

Poly-Gated HfSiON / SiON

UTA Noise and Reliability Laboratory

- NtHK0 values extracted using the MSUN Model
- Shows consistency over the whole experimental temperature range
- Shows consistency with devices having different IL thickness

Poly-Gated HfSiON / SiON

UTA Noise and Reliability Laboratory

Poly-Gated HfSiON / SiON

The active trap densities as

probed by the quasi-Fermi

energy and it’s excursion is

shown for devices with

different IL thicknesses.

As the excursion range is

comparatively small, the

calculated trap density out-

side the highlighted region

may not correctly represent

actual device characteristics.

At 300K, the active trap

density was observed to be

IL dependent. The thinnest

gate oxide devices showed

highest active trap density.

UTA Noise and Reliability Laboratory

- The temperature dependence of extracted trap density is inconsistent with the core model assumption.
- Multi-Stack Unified Noise (MSUN) model is proposed to predict noise in high-k/interfacial layer MOSFETs.
- It is scalable with respect to HK/IL thicknesses, temperature and applied bias.
- It accounts for the material properties of constituent dielectric materials and the non-uniform dielectric trap density profile with respect to energy and location in dielectric.
- Four model parameters
- Mid-gap trap density at the IL/high-k interface
- Parameter for the energy distribution of traps in the high-k dielectric layer
- Spatial trap distribution parameter for the high-k layer
- Mobility fluctuation coefficient

UTA Noise and Reliability Laboratory

- The model is in excellent agreement with the experimental data down to cryogenic temperatures.
- Metal-Gated HfO2/SiO2 NMOSFETs – different interfacial layer processing
- Poly-Gated HfSiON/SiON NMOSFETs – variable interfacial layer thickness
- Metal-GatedHfSiON/SiON MOSFETs – different nitridation techniques

UTA Noise and Reliability Laboratory

Acknowledgements

- Thanks to
- Luigi Colombo, Texas Instruments
- Keith Green, Texas Instruments
- Ajit Shanware, Texas Instruments
- Hsing-Huang Tseng, Freescale
- Ania Zlotnicka, Freescale
- Manuel Quevedo-Lopez, Texas Instruments / SEMATECH

UTA Noise and Reliability Laboratory